Failure Analysis of Natural Gas Pipes
Embed Size (px)
Transcript of Failure Analysis of Natural Gas Pipes
Engineering Failure Analysis 17 (2010) 818837
Contents lists available at ScienceDirect
Engineering Failure Analysisjournal homepage: www.elsevier.com/locate/engfailanal
Failure analysis of natural gas pipesZ.A. Majid a,*, R. Mohsin a, Z. Yaacob a, Z. Hassan ba b
Gas Technology Centre, Universiti Teknologi Malaysia, 81310 Johor, Malaysia Faculty of Chemical & Natural Resources Engineering, Universiti Malaysia Pahang, 26300 Pahang, Malaysia
a r t i c l e
i n f o
a b s t r a c tIncident involving failures of 6 months old API 5L X42 (NPS8) and SDR 17, 125 mm medium density polyethylene pipe (MDPE) supplying natural gas to an industrial customer has caused serious 7 h supply disruption. Study was performed to identify the most probable cause of the pipes failures. The study conducted by reviewing the existing design and construction data, visual physical inspection, pipe material analysis, structural analysis using NASTRAN and Computational Fluid Dynamics analysis (CFD) using FLUENT. Investigations revealed that high pressure water jet from leaked water pipe had completely mixed with surrounding soil forming water soil slurry (high erosive properties) formed at a close vicinity of these pipes. Continuous impaction of this slurry upon the API 5L X42 pipe surface had caused losses of the pipe coating materials. Corrosion quickly ensued and material loss was rapid because of the continuous erosion of oxidised material that occurred simultaneously. This phenomenon explains the rapid thinning of the steel pipe body which later led to its failure. Metallurgical study using photomicrograph shows that the morphology of the steel material was consistent and did not show any evidence of internal corrosion or micro fractures. The structural and CFD simulation results proved that the location, rate and the extent of erosion failures on the pipe surfaces can be well predicted, as compared with actual instances. 2009 Elsevier Ltd. All rights reserved.
Article history: Received 15 July 2009 Accepted 9 October 2009 Available online 15 October 2009 Keywords: Pipeline Slurry erosion Erosioncorrosion Natural gas pipe Failure analysis
1. Introduction Cases involving failure of pipes carrying highly combustible fuel such as natural gas are rarely reported. High pressure natural gas transmission pipeline (API 5L X60) in northern part Pakistan  and a T-shape natural gas pipeline network (API 5L X52) near gas extraction plant in northern Mexico  are two examples of such cases. In both cases the material degradation causes by corrosion is the main factor that contribute to the failure of the pipes. Another example of a similar pipes but carrying liquid fuel that has failed are the 52 km 1600 (406.4 mm) pipe (API 5L X52) in Kuwait  and the API 5L X46 pipe in Brazil . Delayed cracking and transverse cracking has been identied as a reason for the pipes to fail. A case involving the failure of natural gas pipes adjacent to water is yet to be reported. A leak of high pressure water pipe in a mixture of soil and sand can create an erosive slurry impact on nearby pipes. Slurry erosion will form by the interaction of solid particles suspended in liquid and a surface which experience losses of mass by repeated impacts of particles . This type of erosion has been reported as the major source of failure of many engineering equipment such as slurry equipment and hydraulic components . This erosive slurry impact will cause metal loss or metal thinning and eventually lead to the pipe failure . This event could trigger much disastrous incident involving re and explosion which could cause loses in term of life and economics [9,10].
* Corresponding author. Tel.: +60 7 5535574; fax: +60 7 5545667. E-mail address: email@example.com (Z.A. Majid). 1350-6307/$ - see front matter 2009 Elsevier Ltd. All rights reserved. doi:10.1016/j.engfailanal.2009.10.016
Z.A. Majid et al. / Engineering Failure Analysis 17 (2010) 818837
2. Background of the incident The location of the gas pipe leak was evident after the personnel from a gas utility company in northern part of Malaysia observed the bubbling of the gas through the watery soil (Fig. 1). Prompt action was taken where the leakages were immediately isolated through valves. A team was later sent to excavate the site at the incident area. This was carried out in order to locate the exact source of the leakage, to rectify and repair the damaged pipes and to make a proper record of the failure or damage for further investigation. Presented in this paper are ndings, probable cause of failure and conclusions concerning the failure of the pipes. 3. Methodology Studies conducted were comprised of four fundamental aspects. First, the background information which caters in the form of design and construction data that provide basic formation for understanding the sequence of events and operational conditions that might have led to the failures of the pipes. This studied was later followed by physical inspection of specimen, recorded photos and subsequent observation of the actual failed pipes sections. This has been conducted in order to locate the actual position and orientation of pipes and to reconstruct the event that lead to the failure. Next, the metallurgical analysis of pipes was performed on the pipe section and its surrounding failure area, followed by nal study on the structural and ow propagation. The structural analysis will provide insight of the stress distribution in the vicinity of the failed pipe section as thinning occurs. Therefore, the location and weakness area can be well predicted. The CFD analysis conducted could provide simulation of graphical velocity and pressure prole of the leakage and bursting analogy. It could also indicate how it might have affected or lead towards the failure of the adjacent pipe/s. 4. Findings and discussion 4.1. Review of background information Upon the discovery of the incident location area, it was evident that three pipes adjacent to each other; a 800 (203.2 mm) steel NPS8 and a 125 mm MDPE natural gas pipes, and a 600 (152.4 mm) asbestos water pipe lying parallel to each other, with all three indicating signs of damage or leak. An electrical cable lying parallel to the pipes with no apparent sign of damage also presence in a close vicinity. The NPS8 and MDPE pipe was carrying natural gas at about 1800 kPa and 345 kPa pressure, respectively, prior to shut down. The asbestos pipe was transporting water with an estimated owing pressure of 1000 kPa (10 bar). The failed NPS8 gas pipe was made of carbon steel manufactured with specication of API 5L X42. It was buried 1.3 m below the ground about 195 mm laterally from the underground water pipe. The water pipe was buried at a similar depth. Slightly above it, at 1.2 m below the surface and at roughly the same distance between the steel pipe and the water pipe, is the MDPE gas pipe (Fig. 2). The thickness of the NPS8, MDPE and asbestos pipe were 5.6 mm, 11.4 mm and 10 mm respectively (see details in Table 1). There were four possible reasons initially given as the possible root cause of the failures, which are: i. Construction defect. ii. Third party damage.
Fig. 1. Surface water splashing due to gas pipe leakages.
Z.A. Majid et al. / Engineering Failure Analysis 17 (2010) 818837
Fig. 2. Relative positions of API 5L X42, 6 in. asbestos and PE pipes.
Table 1 Physical parameters of pipes. Parameters Depth cover (m) Material Internal diameter (mm) External diameter (mm) Thickness (mm) Fluid pressure (KPa) NPS8 gas pipe 1.3 Carbon steel 203.2 214.4 5.6 1800 PE gas pipe 1.2 Polyethylene 102.2 125.0 11.4 345 Water pipe 1.3 Asbestos 152.4 172.4 10.0 1000
iii. Pipeline material defect. iv. Leaking water pipe impact. It is made to understand that the pipeline was laid about six months prior to the incident. Standard construction procedures that require proper coating, sound cathodic protection system and other pipeline integrity measures has been appropriately complied during construction and pipe laying process. This diminished the possibility of the construction defects. On the possibility of third party works or acts, initial discussion with the gas utility company personnel and available operational records dismissed that this had taken place. Furthermore, visual inspection did not nd any indication or evidence to support this fact. To answer the third possibility, the metallurgical analysis was subsequently performed and will be discussed details in the following section. Visual inspections were carried out on both the photos and on the two physical pipe specimens provided (Fig. 3). When received, the exposed part of the steel pipe (with the coatings eroded) is already heavily oxidized (Figs. 3a and 4a). Only when the photo records were received, was the original condition of the exposed part, immediately after the incident, became evident. It was found that the coating materials has been completely stripped was in fact clean, smooth and shiny (Fig. 4b). The pipes were later rearranged in the lab to reconstruct the positioning of each pipe relative to each other prior to the failures. This was conducted based on the original information supplied. The repositioning of the pipes was important to help us to build a better understanding on the direction of the leaks and how it might have impacted upon the adjacent pipes (Fig. 5). On the NPS8 carbon steel pipe section, a hole with an average diameter of 10 mm was discovered in the middle of the eroded part of the pipe (Fig. 6). The eroded part was found to be smooth and free from the rust. The size of the eroded section was around 50 cm by 30 cm (Fig. 4b). The absence of scratch marks or dents in the vicinity of the eroded part seem to support the statements of site engineers that no third pa